Systematic Evolution from Uranyl(VI) Phosphites to Uranium(IV) Phosphates
Eric M. Villa; Connor J. Marr; Laurent J. Jouffret; Evgeny V. Alekseev; Wulf Depmeier; Thomas E. Albrecht-Schmitt; Inorganic Chemistry 51 (2012) 6548–6558; doi:10.1021/ic3000735

data_4329430
_publ_section_title
;
 Systematic Evolution from Uranyl(VI) Phosphites to Uranium(IV) Phosphates
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6548
_journal_page_last               6558
_journal_paper_doi               10.1021/ic3000735
_journal_volume                  51
_journal_year                    2012
_chemical_formula_moiety         Cs2[UO2(HPO3)(H2PO3)]2
_chemical_formula_sum            'Cs2 H4 O16 P4 U2'
_chemical_formula_weight         1125.79
_chemical_name_common            'Room Temp - Cesium Uranium(VI) Phosphite'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                94.147(3)
_cell_angle_beta                 95.880(3)
_cell_angle_gamma                90.411(4)
_cell_formula_units_Z            2
_cell_length_a                   7.9754(11)
_cell_length_b                   10.5635(15)
_cell_length_c                   10.6772(15)
_cell_measurement_reflns_used    5308
_cell_measurement_temperature    103(2)
_cell_measurement_theta_max      30.86
_cell_measurement_theta_min      1.92
_cell_volume                     892.4(2)
_computing_cell_refinement       'smart saint'
_computing_data_collection       smart
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXP-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXCIF-97 (Sheldrick, 2000)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      103(2)
_diffrn_detector_area_resol_mean 0
_diffrn_measured_fraction_theta_full 0.942
_diffrn_measured_fraction_theta_max 0.942
_diffrn_measurement_device_type  'BRUKER apex II'
_diffrn_measurement_method       '0.5 wide w/ exposures'
_diffrn_radiation_monochromator  'Quazar optics'
_diffrn_radiation_source         'Imus microfocused'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0457
_diffrn_reflns_av_sigmaI/netI    0.0453
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            19540
_diffrn_reflns_theta_full        30.86
_diffrn_reflns_theta_max         30.86
_diffrn_reflns_theta_min         1.92
_exptl_absorpt_coefficient_mu    22.574
_exptl_absorpt_correction_T_max  0.569
_exptl_absorpt_correction_T_min  0.352
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   SHELTXPREP
_exptl_crystal_colour            Yellow-Green
_exptl_crystal_density_diffrn    4.190
_exptl_crystal_density_meas      ?
_exptl_crystal_description       Block
_exptl_crystal_F_000             972
_exptl_crystal_size_max          0.050
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.025
_refine_diff_density_max         4.851
_refine_diff_density_min         -3.113
_refine_diff_density_rms         0.289
_refine_ls_extinction_coef       N/A
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.038
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     229
_refine_ls_number_reflns         5308
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.038
_refine_ls_R_factor_all          0.0395
_refine_ls_R_factor_gt           0.0312
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0262P)^2^+3.2222P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0669
_refine_ls_wR_factor_ref         0.0696
_reflns_number_gt                4490
_reflns_number_total             5308
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic3000735_si_002_3.cif
_cod_data_source_block           RT_Cs_U(VI)_PO3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'N/A' was changed to '?' - the
value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_database_code               4329430